Degree Thesis Flexural Rigidity (D) in Beams. Author: Zious Karis. Instructor: Rene Herrmann


 Amber Marsh
 1 years ago
 Views:
Transcription
1 Degree Thesis Flexural Rigidity (D) in Beams Author: Zious Karis Instructor: Rene Herrmann Degree Thesis Materials Processing Technology 2017
2 DEGREE THESIS Arcada University of Applied Sciences, Helsinki, Finland Degree Programme: Identification number: Author: Title: Supervisor (Arcada): Materials Processing Technology Zious Karis Flexural Rigidity in Beams Rene Herrmann Commissioned by: Abstract: This thesis presents the theory behind the symmetrical and unsymmetrical beams with different crosssections, the mathematical procedure in calculating the flexural rigidity of symmetrical beams and summarizing the experimental verification by mathematical data processing of the flexural rigidity by threepoint bending. The core of the method section is to test theoretically by using the composite compressive strength modeler (CCSM) software and experimentally in the laboratory by using the material bending machine a solid fiberglass and a sandwich beam. The results obtained for the solid fiberglass was found to be theoretically 32 Nmm 2 and experimentally 31.1 MNmm 2. For the sandwich beam along the direction of the orientation of the fiber theoretically 155 Nmm 2 and experimentally Nmm 2. As for the sandwich beam with the same properties but with a direction perpendicular to the fiber theoretically 45.1 Nmm 2 and experimentally Nmm 2. The comparison of flexural rigidity values was found to be 3.1% for the solid fiberglass, 1.1% for the sandwich beam along the direction of the orientation of the fiber and 4.6% with a direction perpendicular to the fiber. Moreover, for the foursection module, the values obtained for the moments of the outer layer contributed seven times more to rigidity than the inner layer and for the sixsection module the second outermost layer contributed seven times more than the innermost layer and the outermost layer nineteen times more to rigidity than the innermost layer. Keywords: Flexural rigidity, deflection in beams, symmetrical bending, sandwich structure, composite beams, (CCSM) modeler, threepoint bending Number of pages: 60 Language: English Date of acceptance: 2
3 CONTENTS 1 INTRODUCTION Problem Definition Aims and Objectives Method Background Flexural Rigidity THEORY Second Moment of Area Materials Composite Materials Composites versus Metallic Bending Stiffness of Beams Theory of Simple Bending with Assumptions Made Bending of Composite Beams Symmetrical Bending Examples of Symmetrical Bending Unsymmetrical Bending History of Sandwich Structure Sandwich Structure Flexural Rigidity in Sandwich Beams Deflection of Beams METHOD Composite Compressive Strength Modeler (CCSM) A Solid UD Lamina Bending ThreePoint & FourPoint Bending RESULTS Bending Test and CCSM Modelling DISCUSSION
4 6 CONCLUSION REFERENCES
5 Figures Figure 2.1 Composite structure [6] Figure 2.2 Steel vs. sandwich [9] Figure 2.3 Strain [11] Figure 2.4 Ibeam [13] Figure 2.5 Rectangular crosssection Figure 2.6 Centroidal xaxis Figure 2.7 Twosections Figure 2.8 Foursections Figure 2.9 Sixsections Figure 2.10 Rectangular beam [15] & Figure 2.11 Upward restoring force [15] Figure 2.12 Tbeam [16] Figure 2.13 Efficiency of sandwich structure [9, p. 256] Figure 2.14 Sandwich structure [18, p. 5] Figure 2.15 Sandwich beam cross section [4] Figure 2.16 Deflection and curvature due to bending [20] Figure 2.17 Cantilever beam [20] Figure 2.18 Simply supported beam [20] Figure 2.19 Simply supported beam, deflection at center Figure 2.20 Simply supported beam, uniformly distributed load Figure 3.1 Principal material axes in a UD lamina [23] Figure 4.1 Materials testing machine Figure 4.2 Solid fiberglass  theoretical Figure 4.3 Solid fiberglass theoretical d Figure 4.4 Solid fiberglass  experimental Figure 4.5 Sandwich beam 1  theoretical Figure 4.6 Sandwich beam 1 theoretical d Figure 4.7 Sandwich beam 1  experimental Figure 4.8 Sandwich beam 2  theoretical Figure 4.9 Sandwich beam 2 theoretical d Figure 4.10 Sandwich beam 2  experimental
6 Tables Table 1. Composites versus metals under certain conditions. [9] Table 2. ASTM standards for threepoint bend. [27] Table 3. ASTM standards for fourpoint bend. [27] Table 4. Values for the CCSM Modeler Table 5. Results
7 List of Symbols Name Symbol Unit 1. Flexural rigidity D Nm 2 2. Bending modulus (material property) E Pa = N/m 2 3. Young s modulus of faces Ef Pa 4. Second moment of inertia I m 4 5. Width b m 6. Thickness t m 7. Distance d m 8. Force F N 9. Height h m 10. Moment/Bending moment M Nm 11. Stress σ Pa = N/m Length L m 13. Area A m Strain Ε  or mm/mm 15. Shear stress Q Pa 16. Slope Θ (k) N/mm 17. Distance along beam x m 18. Radius of neutal axis r m 19. Distance of surface (NS) y m 20. Torque τ Nm 21. Deflection Y mm 22. Distributed load W N/m 7
8 FOREWORD I would like to thank Mr. Rene Herrmann for the supervision throughout this thesis. I would like to thank all the professors and staff for their guidance during my three years of studying at Arcada University of Applied Sciences. Special thanks to Mr. Erland Nyroth for his encouragement and advices throughout my studies. Finally, I would like to thank my family and friends for their continued support over last few years, particularly during the completion of this thesis. Special thanks to my father for his unlimited support and encouragement. Special thanks also to Mr. Manuel Eisenbarth for his unlimited support and help especially over the thesis time. 8
9 1 INTRODUCTION The purpose of this thesis work is to summarize the mathematical procedure to calculate the bending stiffness of symmetrical and unsymmetrical beams with different cross sections such as I, Rectangular, and Tcrosssections. This paved the way for the summary of the experimental verification by mathematical data processing of the flexural rigidity by 3point, a review on composites and metals as well the comparison between them. Moreover, it is intended to summarize on some examples the theoretical and experimental flexural rigidity and to review international measurement standards for polymer and composite materials, finally, using the CCSM (Composite Compressive Strength Modeler) for deformation analysis of composite materials. 1.1 Problem Definition Structural efficiency is one of the most important character to engineers in the aerospace, boats, car industries and in many other fields. Therefore, a highperformance product made of lightweight materials and yet efficient to withstanding harsh loading conditions is required. The stiffness as a material property is very important in structural engineering as it extents the materials resist deformation in response to applied load. The use of sandwich composites has been considered in this thesis due to the relevance of its stiff light weight structure, which significantly increases the load resistance capacity on one hand without much increase in weight on the other hand. To design a member such as a beam, it is very essential to make sure that it satisfies specific strength, stability, and deflection requirements. Therefore, the bending stiffness analysis plays a major role in choosing materials as it shows how a component behaves under certain loads. 9
10 1.2 Aims and Objectives In order to fulfil the aim of this thesis, the research is conducted aiming to calculating mathematically the flexural rigidity of symmetrical cross sections, verify the experimental results of mathematical data processing of the flexural rigidity by 3point bending, present some examples to illustrate the theoretical and experimental flexural rigidity, review of verification methods for 4point bending, comparing composite materials to metals using some international measurement standards and using composite compressive strength modeler (CCSM) software for modelling of flexural rigidity. 1.3 Method In order to achieve the aim of this thesis and get the theoretical knowledge of the problem, the theory of bending stiffness for different beams and plates have been studied. In the consideration of the bending stiffness analysis of composite material structures, the composite compressive strength modeler (CCSM) and experiments on different materials in the laboratory have been conducted. There are several software packages available for rigidity analysis and deformation tests. In this thesis work, the composite compressive strength modeler (CCSM) software is used for flexural rigidity simulation. 1.4 Background Flexural rigidity is related to bending and nonrigid structures as a force couple that is required to bend a nonrigid structure in one unit of curvature, where force couples also known as pure moments are the forces that rotate a body without translation or acceleration of the center of mass. [1] Since force couples are free vectors in rigid bodies, their effects on a body are independent of the point of application. A couple is known as a combination of two forces, they are equal in magnitude, asymmetrically directed, and displaced by a perpendicular distance or moment. [1] 10
11 1.4.1 Flexural Rigidity Flexural rigidity can be modelled by using different methods. In this scientific discourse, three of the very wellknown methods in the bending stiffness of a profile are treated. The first method can be applied when the modulus is constant, and the cross section is simple then the single formula of second moment of inertia (equation 2, p.12) can be used to obtain the required results of flexural rigidity D. [2] The second method is used when the modulus is constant, and the cross section is not simple but can be however reduced to a simple cross section with a displacement from the neutral axis, in this case the parallel axis theorem can be used effectively by determining the second moment of area or mass moment of inertia of a rigid body about any axis. [3] While the third method which is known as the sandwich beam theory or the Euler Bernoulli beam theory that describes the behavior of a beam, plate, or a shell when calculating the loadcarrying and deflection characteristics of beams. It is used when the profile is not constant in bending modulus, but the profile can be approximated or considered as a layered structure of different materials. [4] The flexural rigidity (D) is defined as EI. In a beam or rod, flexural rigidity varies along the length as a function of (x): Where, x EI dy dx = M(x)dx + C 1 0 (1) [1] E = Young s modulus (Pa) I = second moment of area (m 4 ) y = transverse displacement at x (m) M (x) = bending moment at x (Nm) 11
12 2 THEORY The Euler Bernoulli s Equation and the bending stiffness of a rigid body expresses clearly the flexural rigidity. [1] Euler Bernoulli is known as an engineer of beam theory, which simplifies the linear theory of elasticity. It provides a calculation for the loadcarrying and deflection characteristics of beams and it covers the case for infinitesimal strains and small rotations of a beam which are only subjected to lateral loads. [5] The theory can be extended in a straightforward manner to problems with moderately large rotations by using the von Kármán strains, which provides that the strain remains small. However, in this thesis work the focus is on bending stiffness. [5] Stiffness describes the rigidity of an object, in other words it is the resistance to deformation when a force is applied on it. So, the flexibility of materials is very essential, the more flexible an object is, the less stiff it is. The stiffness of a body is a measure of the resistance offered by an elastic body to deformation. The bending stiffness of a beam is a function of elastic modulus E, the area moment of inertia I of the beam crosssection about the axis of interest, length of the beam and the beam boundary conditions. The bending stiffness of a beam can be analytically derived from the equation of beam deflection when it is applied by a force. [1] 2.1 Second Moment of Area Second moment of area is the property of a cross section. It is normally used to predict the resistance of beams to bending and deflection. The deflection of beams under a certain load doesn t depend only on the load but also on the geometry of the beam s cross section. Beams with a large second moment of area are stiffer than those with a smaller second moment and therefore, they are more resistant to bending. The second moment of area has in other words the meaning of second moment of inertia: [2] I = I 0 + Ad 2 (2) [2] Where, I = second moment of inertia (m 4 ) I0 = second moment of area at centroidal axis (m 4 ) 12
13 A = area (m 2 ) d = distance (m) 2.2 Materials Nowadays, the designing of materials and material properties play a big role in the development of materials. However, there are two main types of materials. The first type is known as structural materials, where the mechanical properties are mainly considered, such as strength, stiffness, and deformation. And the second type is known as functional materials where, the magnetic properties are mainly considered, such as the sound, light, electricity, and heat. [6] Moreover, these materials can be divided into three types depending on the way the atoms or molecules are bonded together. Metallic materials describe the first type, where metal elements are combined with metal bonds, organic polymer materials stand for the second type, where nonmetallic elements are bonded covalently to macromolecular compounds while ceramic materials describe the third type, where nonmetallic elements and metal elements are combined by covalent bonds, ionic bonds, or a mixture of the two bonds. [6] Composite Materials Composite material also known as a multiphase combination material. Composites are formed by combining materials together to form an overall structure with properties that differ from the sum of the individual components. [7] They are generally used for buildings, bridges, and structures due to their benefits such as chemical and corrosion resistance, durable, flexible in design, high flexural modulus to carry demanding loads, high impact strength, high performance at elevated temperature, etc. [7] Composite materials consist of matrix material and reinforcing material as shown in figure 2.1 below, where matrix materials are defined as a continuous phase, which includes metal matrix composite materials, inorganic nonmetallic matrix composite materials as well polymer matrix composites by the different matrix material. Reinforcing material is defined as a dispersed phase which includes usually fibrous materials, such as glass fiber, and organic fiber. [6] 13
14 Figure 2.1 Composite structure [6] Normally the strength of fiber depends on its length and orientation with respect to the stress direction, however, the strength and modulus of fiber are much higher than the matrix material, due its length and accordingly the orientation of stress direction therefore, fibers are the main loadbearing components. However, to firmly bond fibers together, there must be a matrix material with good adhesion properties that can provide a uniformly distributed applied load and transfer the loads to fiber. [6] Composite materials should have at least four characteristics. The composite should be made of a nonhomogeneous material, the components that make up the composite should have different levels of performance, the performance should be the main characteristic of all composites, and the fraction of each component of the composites should be larger than 10 percent of the volume of the composite. [6] Composites versus Metallic Composites and metals have different physical characteristics. For instance, composites are greatly anisotropic which means their properties and values are changeable with direction as well as their strength and stiffness, depending on the orientation of the reinforcing fibers. [8] In addition, composites are lighter in weight, they can tailor the layup for optimum strength and stiffness, improve fatigue life, corrosion resistance, etc. While the metals are isotropic which means their physical properties have the same values in different directions, they are much heavier than composites in weight. Figure 2.2 and table 1 below illustrate an example of some main differences between a composite and a metal. [8] 14
15 Figure 2.2 Steel vs. sandwich [9] Table 1. Composites versus metals under certain conditions. [9] Condition Loadstrain relationship Static Fatigue Transverse properties Mechanical property Fatigue strength Sensitivity to hydrothermal Sensitivity to corrosion Damage growth mechanism Comparative behavior relative to metals More linear strain to failure Greater sensitivity Less sensitivity Weaker Higher Higher Greater Much less Inplane delamination instead of through thickness cracks 2.3 Bending Stiffness of Beams This section covers some concepts about the bending stiffness of symmetrical and unsymmetrical beams with different cross sections, the study of simple bending, and bending of composite beams Theory of Simple Bending with Assumptions Made Simple bending happens at the length of a beam that is subjected to a constant bending moment and when there is no shear force, that is (Q = 0). Which means that the stresses will be arranged along the length of the beam, due to the bending moments only. Therefore, that length of the beam is said to be in pure bending. The assumptions made in the theory of simple bending are known as, the beam is homogeneous and isotropic, the Young s modulus of elasticity in tension and 15
16 compression has the same value, the transverse sections which were plane before bending remain plane after bending, the beam at the beginning of the experiment is straight, and all longitudinal filaments bend into circular arcs with a common center of curvature, the radius of curvature is large compared with the dimensions of the cross section, and each layer of the beam is free to expand or contract, independently of the layer above or below it. [10] However, there are some other tools to use for complicated designs such as a superposition principle or property tool. This tool is used in linear systems for the beams. The superposition principle is one of the most important tools for solving beam loading problems as it allows the simplification of very complicated designs. [10] For the beams that are subjected to several loads of different types the resulting shear force, bending moment, slope and deflection can be found at any location by summing the effects due to each load acting separately to the other loads. The superposition principle is a combination of homogeneity and additivity and satisfies the following equations. [10] Additivity: Homogeneity: F(x 1 + x 2 ) = F(x 1 ) + F(x 2 ) (3) [10] F(ax) = af(x) (4) [10] Simple bending is when a straight bar of homogeneous material is subjected to only a moment at one end and an equal and opposite moment at the other end Bending of Composite Beams A composite beam is made of two or more different materials where these materials are connected rigidly, and the composite behaves like a single piece once it is made. The basic assumption in this case assumes that the plane surface remains plane during bending within the elastic limit [10]. Therefore, the strain remains constant down at the full width of the beam, where the deflection is proportional to the distance from the neutral axis of the beam, in this case the strain can be found easily, and it is equal to (stress/young s Modulus E) [11]. As shown in figure 2.3 below. 16
17 Figure 2.3 Strain [11] The dimensions of the replacement material have the same mechanical properties as the original material, and the overall depth of the transformed section is the same as the original section. Therefore, the resulting strain in any element da of the transformed section must be constant. [11] Strain (ε) = σ (5) [11] E Where, ε = strain (mm/mm) σ = stress (N/m 2 ) E = bending modulus (material property) (Pa) The bending stresses of a composite beam can be calculated using two conditions as follows. [10] 1. The resulted strain on a layer with an equal distance from the neutral axis is the same for both materials. σ 1 E1 = σ 2 E2 σ 1 = σ 2 ( E 1 E 2 ) = mσ 2 (6) [10] 2. The moment of resistance of a composite beam can be determined simply by summing up the individual moments of resistance of the members. M = M 1 + M 2 (7) [10] 17
18 M 1 = σ 1 ( I 1 y ) M 2 = σ 2 ( I 2 y ) M = σ 1 y I 1 + σ 2 y I 2 Where, σ = stress (N/m 2 ) E = bending modulus (material property) (Pa) M = bending moment (Nm) I = moment of inertia (m 4 ) y = distance (m) m = modular ratio, which means in construction the ratio of Young s Moduli of elasticity of the two different materials. (N/m 2 ) Symmetrical Bending The symmetrical bending can be defined as a bending where the bending moments are symmetrical around the neutral axis that passes through the center. Symmetrical bending mainly happens in beams that have symmetrical cross section which can be either single or double layers. [11] The second moment of area which is needed in calculations of bending in beams and also known as the moment of inertia of a shape, it depends on the geometry of objects and it describes how points or particles of an object or an area are distributed about an axis that can be chosen arbitrarily. [11] Examples of Symmetrical Bending One of the examples of symmetrical bending is an Icrosssection beam. Tension and compression loads are applied to the flanges and the body (web) is the core that keeps the facings in place by resisting transverse shear loads. [12] The second moment of area is very high in Isection beam because most of its material is located in the flanges which are placed far from the center of bending (neutral axis), 18
19 and the web has enough material that makes the flanges work together and resist shear and buckling. [12] There are different ways to calculate the bending stiffness of beams. However, for the following shape as an example and since the beam is symmetric from the top to bottom, there is no need to find the centroid of the location. [13] Figure 2.4 Ibeam [13] As it shows from the figure 2.3 above, the I cross section consists of three pieces, instead of treating each piece separately and making separate calculations. It is valuable to treat the whole beam as a rectangle and as a total solid cross section which can be divided into two symmetrical pieces around xaxis and since the centroids of all segments lie on xaxis, there is no need to use the parallel axis theorem. [13] So, the solution for this particular example can be obtained using the following simple moment equation. I x = 1 12 b centerh 3 center The flexural rigidity can be determined from equation 1 page 13. (8) [13] However, in the case of taking all three pieces into consideration, knowing that the beam is symmetric and the center of gravity in the middle then the flexural rigidity D is: [1] D = D i = E(I top + I bottom + I center ) (9) Considering that, [13] I center = 1 12 b 3 centerh center 19
20 And for the bottom and top parts, there is a distance d from the neutral line, so the moment is: [3] I = I center + Ad 2 I top = 1 12 b 3 toph top + b top h top d 2 Where the displacement d is: And the area A is: Since it is symmetric then: d = h center 2 A = b top h top I top = I bottom + h top 2 Another wellknown example of a symmetrical bending is a rectangular cross section beam. The calculation in this case can be done in different ways, one way is by finding the second moment of inertia of the area of a structural section and using the parallel axis theorem. Another common way used in calculations is known as section modulus method. An explanation of both methods is discussed below. [12] 1. Parallel Axis Theorem: In this method a rectangular cross section beam that has a width b and height h is considered as shown in figure 2.4 below. Figure 2.5 Rectangular crosssection Then the area A is: A = b h (10) [12] 20
21 And the moment of inertia I around xaxis that passes through the centroid of the rectangle is: I = 1 12 bh3 And it can be used to calculate the flexural rigidity as follows: [12] D = E I = E 1 12 bh3 When the rotation is around an axis at a distance d from xaxis and is parallel to the centroidal axis as shown in figure 2.6 below. Figure 2.6 Centroidal xaxis Then we use the following parallel axis theorem: [3] I x = I x + Ad 2 2. Section Modulus Method: In this method the crosssection beam is considered to be symmetric from top to bottom, so there is no need to find location centroid. Therefore, the entire rectangle is taken as a total solid cross section and divided into many sections. However, in this thesis work two, four, and six sections are considered below. [13] TwoSection Modulus: In this case a rectangular beam is cut into twosection modulus as in figure below. 21
22 Figure 2.7 Twosections The moment of inertia for each element from top to bottom in this case can be obtained first and then summing up to get the main moment I which can be used to calculate the flexural rigidity as below: For each element top or bottom: [3] Where, I = I 0 + Ad 2 A = b h 2 d = h 4 I 0 = 1 12 b (h 2 ) 3 b = width (m) h = height (m) The moment of inertia for the upper part of the beam is found by substituting A and r into moment equation so we get: I up = 1 12 b (h 2 ) 3 + b ( h 2 ) (h 4 ) 2 I up = 1 96 bh3 + bh And the moment of inertia for the bottom part is determined by substituting the same A and r values into the moment equation again, taking into consideration the negative sign of d, that is (d). So, we get: 22
23 I down = 1 12 b (h 2 ) 3 + b ( h 2 ) ( h 4 ) 2 I down = 1 96 bh3 + bh Then the total moment I is the sum of top and bottom moments: I tot = I up + I down = 2I = bh ( ) 2 = bh 3 ( ) 2 = bh So, the flexural rigidities can be calculated when E, b, h are given and as follows: D = E I tot D = E (bh ) FourSection Modulus: In this module the beam is divided to four sections, the individual moments are calculated in a similar way to the twosection modulus and then the total moment is substituted in the equation of flexural rigidity. The figure 2.8 below illustrates the sections and dimensions used in calculations. Figure 2.8 Foursections For each element top or bottom: [3] I = I 0 + Ad 2 23
24 Where, A = b h 4 That leads to, d = h 8 I 0 = 1 12 b (h 2 ) 3 The first moment I 1 can be obtained by substituting these values into the following equation: I 1 = I 0 + Ad 2 = 1 12 b (h 2 ) 3 + bh 4 (h 8 ) 2 I 1 = bh 3 ( ) = bh 3 ( ) For I 2 an additional distance of ( h ) which is 4 (h) + 8 (h ) is considered in calculations as 8 shown below: I 2 = b (h 4 ) + bh 4 (h 4 + h 2 8 ) = 1 h3 b b h 2 4 (3h 8 ) I 2 = bh 3 ( ) The moments I3 and I4 can be obtained in the same way and then Itotal which is the sum of the moments of all elements is substituted in the flexural rigidity equation 1 page 13. Moreover, the moments related to the thickness t can be calculated in a similar way. The general formula for the moment I in this case is: So, for I 1 with thickness t1 we get: I = 1 12 b(4t)3 = bt (11) [3] 24
25 I 1 = 1 12 bt bt ( t 2 ) 2 And for I 2 we get, I 2 = 1 12 bt bt ( t 2 ) 2 For the first and the second moment I 1/2 we get, I 1/2 = b ( 1 12 t3 + t ( t 2 ) 2 ) 2 I 1/2 = bt 3 ( ) 2 = bt3 ( ) 2 I 1/2 = bt In a similar way the third and the fourth moments are obtained and then we get I 3/4 : I 3/4 = b ( 1 12 t3 + t ( 3 2 t) 2 ) 2 I 3/4 = bt 3 ( ) 2 = 4 + (9 12) bt3 ( ) 2 48 I 3/4 = bt = bt So, I total is: I tot = I i = I 1/2 + I 3/4 = bt3 24 (128) I tot = bt It can be seen from the values obtained for the moments of the outer and the inner layers, that is values of I 1/2 and I 3/4 that the outer layer contributes seven times more to the rigidity than the inner layer, since the ratio of the outer and the inner layer is: = 7 25
26 SixSection Modulus: In this symmetric six section module, the moments for three layers will be considered and calculated and then generalize the results to the other three since the module is symmetric as shown below. Figure 2.9 Sixsections For each element top or bottom: Where, I = I 0 + Ad 2 A = b ( h 6 ) And the three distances are: d 1 = h d 2 = h 6 + h 12 d 3 = h h 12 Applying the general moment equation below: I = 1 12 b (h 6 ) 3 + b h 6 ( h 12 ) 2 (12) [2] 26
27 Then we get I 1 : I 1 = bh 3 ( 1 12 (1 6 ) ( 1 12 ) 2 ) = bh 3 ( ) = bh And for I 2 we get: I 2 = b (h 6 ) + b ( h 2 6 ) (3h 12 ) I 2 = bh 3 ( 1 12 (1 6 ) (1 4 ) 2) = bh 3 ( ) = bh In the same way I 3 : I 3 = 1 12 b ( (h 6 )3 + b ( h 6 ) ( 5 12 h)2 ) I 3 = bh 3 ( 1 12 (1 6 ) ( 5 12 ) 2 ) = bh 3 ( ) = bh The ratios of I 2 and I 1 the outer and the inner layers are: 7 1 = 7 The second outermost contributes seven times more to rigidity than to the innermost. The ratios of I 3 and I 1 the outer and the inner layers are 19 1 = 19 27
28 And the outermost contributes nineteen times more to rigidity than the innermost. From the results and as a conclusion, it can be seen that the outer moments are also dominating in this case by comparing the obtained values of I1, I2, and I3 which gives a clear idea that the rigidity is higher at outer layers, according to the equation of flexural rigidity. It should be mentioned that in a rectangular cross section the contact force and deflections are of great importance, especially when the contact force is directly proportional to the area moment of inertia I of the cross section, where the elastic modulus of the beam material and the beam geometry play a big role in the amount of stress and applied force. So, for instance when the beam is pushed down, there will be an upward restoring force which is equal in magnitude but in opposite direction to the applied force as shown in figure 2.11 below. [14] Figure 2.10 Rectangular beam [15] Figure 2.11 Upward restoring force [15] These forces, deflection, yield, and maximum deflection can be calculated according to the following formulas. Contact Force: F = [ E w t 4 L 3 ] d (13) [14] Deflection at the yield: Y yield = 2 L 2 3 E t σ yield (14) [14] Maximum deflection at load: Y = Fl3 48EI (15) [14] 28
29 Contact force at yield: F yield = [ E w t3 4 L 3 ] d yield (16) [14] = [ E w t3 4 L 3 ] [ 2 L2 3 E t ] σ yield Where, Y = deflection (mm) d = distance (m) F = force (N) σ = stress (N/m 2 ) L = length (m) t = thickness (m) w = b = width (m) I = area moment of inertia (m 4 ) E = bending modulus (material property) (Pa) For known parameters such as dimensions, applied force, and other parameters then the maximum deflection at load for instance can be calculated from equation 19 by using flexural rigidity equation. Which shows the importance of flexural rigidity when studying deflection, contact force at yield, deflection at yield, etc Unsymmetrical Bending In the case of nonsymmetrical section, the neutral axis doesn t pass through the center of the geometrical section. So, the value of y which is the distance of the layer from the neutral axis varies for layers that are located for example at the top and bottom of the section. In order to calculate the bending and since the module is unsymmetrical, the center of gravity of the sections must be found first. [10] The center of gravity (Cg) is defined to be the center to an object s weight distribution, where the gravity force is considered. It is the point where the object is balanced completely, regardless of point of rotation or turning around. Knowing that the neutral axis normally passes through the center of gravity of the section, so by calculating the 29
30 center of gravity of the section, one can find the y values for topmost layer as well for the bottom layer of the section. [10] To more explain the unsymmetrical module, a Tcrosssection example is studied. The top part of the slab is called flange which resists the compressive stress and the part that lies below the slab is called rib which resists the shear stress. [10] Figure 2.12 Tbeam [16] To find the moment, the centroid X and y of a Tsection are calculated first: X = a 1x 1 + a 2 x 2 a 1 + a 2 (17) [16] y = a 1y 1 + a 2 y 2 a 1 +a 2 (18) [16] Where, a1 and a2 are the areas of the flange and rib respectively. The second moment Ixx is: [16] I xx1 = 1 12 W 1H a 1 k 3 2 I xx2 = 1 12 W 2H a 2 k
31 I xx = I xx1 + I xx2 Where, k i = Radius of gyration k 3 = y y 1 To calculate Iyy: [16] k 4 = y y 2 I yy1 = 1 12 W 1H a 1 k 1 2 I yy2 = 1 12 W 2H a 2 k 2 2 I yy = I yy1 + I yy2 Where, k i = Radius of gyration k 1 = x x 1 k 2 = x x 2 So, the flexural rigidity is obtained as in previous sections by substituting the total moment I in the rigidity formula. 2.4 History of Sandwich Structure According to [17]. Delau in England introduced the first sandwich construction, back to Fairbairn The first use of sandwich panels aircraft sandwich was used in World War II. Mainly because of the lack of other materials during the war. The Sandwich Structure theoretically appeared in the 50 s. The use of sandwich structure had some limitation in aircraft industry as honeycomb was mainly used as core material and there were big problems with corrosion due to water absorption, UVRadiation, aging etc. [4]. Figure 2.14 below illustrates the Sandwich Structure efficiency. 31
32 Figure 2.13 Efficiency of sandwich structure [9, p. 256] However, during the early 60 s, there was a production of different cellular plastics which were suitable as core materials. Soft materials were used in the beginning because of their insulation properties such as polystyrene and polyurethane. Later sandwich structure became very useful and flexible concept as harder cellular plastics with higher densities were possible to produce caused by diverse progresses in material production. [17] Nowadays, there is an enormous number of different qualities of cellular plastics that are used as core materials. Sandwich panels became an important composite structure in aerospace applications as well as in high performance automobiles, boats, and wind turbines, because it is an extremely lightweight type of construction that exhibits high stiffness and high strengthtoweight ratios. [4] Sandwich Structure The importance of studying and analyzing these structures is growing as mentioned in the history of sandwich structure. The calculation for flexural rigidity and other quantities can be seen clearly when considering a sandwich structures as they are a suitable example of composites. Sandwich structure consists of two stiff, strong faces separated by a lightweight core and joints (adhesives), which can be seen in figure 2.14 below. [4] 32
33 Figure 2.14 Sandwich structure [18, p. 5] Facing sheets of a typical sandwich structure are mainly thin with a relatively thick lightweight core that separates the two faces in order to increases the moment of inertia. It is for important for engineers or designers of sandwich structures to make the core strong enough to withstand heavy loads and keep their positions. [9] Each component of the sandwich structures has some specific properties that make the sandwich function effectively as a oneunit object. It is preferred by engineers to make the faces of the sandwich structure from some very wellknown metals such as steel, stainless steel, or aluminum due to their stiffness and strength, due to the fact that these materials have some special mechanical properties and they are uncomplicated to use and fabricate. However, in some cases fiber  reinforced plastics are used as face materials as well, because they have good physical properties such as strength. [17] The core has several critical capacities. It must be sufficiently stiff to keep the separation between the faces steady and it must be so rigid in shear to prevent the faces from sliding over each other. The core must be strong in shear to keep the faces cooperating with each other, if the core is weak in shear, the sandwich loses its stiffness. To keep the faces and the core cooperating with each other, the adhesive layer must be added as it enables the transmission of the shear forces between the faces and the core. The adhesive must have the capacity to carry shear and tensile stresses. [4] Flexural Rigidity in Sandwich Beams Since sandwiches are composites and according to their properties, engineers managed to modify and adjust the beam theories so that they can be applied to the sandwich structures and can be used in analyzing and calculating flexural rigidity of sandwiches. [4] 33
34 Figure 2.15 Sandwich beam cross section [4] For beams, the sandwich is slightly different, and it consists of a few different parts where the entire section should be considered when measuring its parts around the centroidal axis. [4] So, the flexural rigidity can be determined as follows: D = Ef ( bt3 6 ) + Ef (btd2) + Ec (bc ) (19) [4] Where, Ef = moduli of elasticity of the faces (index f) Ec = moduli of elasticity of the core (index c) Equation 22 above consists of three terms that calculates flexural rigidity depending on the local flexural rigidity of the faces about their own centroidal axes, bending about the centroidal axis of the entire cross section and the flexural rigidity of the core about its own centroidal axis. [4] When this equation is applied to a sandwich structure and comparing the results to the results obtained earlier for a sixsection modulus found in page 2829, it can be seen that the sandwich is a special case of a sixlayer parallel axis theorem. According to some studies and experiments on sandwich structure with thin faces, engineers and scientist concluded that the amount of flexural rigidity due to faces around their own centroidal axis is very small (less than 1%) compared to the rigidity of the bending of the entire cross section around the centroidal axis, therefore it can be neglected especially when: d t >
35 And the proportion is less than 0.25% at a ratio of: d t > Since the faces are thin, not only the first term can be ignored but in fact experiments showed that the third term of equation 28 is also very small (less than 1%) of the second term which means that it can be ignored as well when: ( E f E c ) ( td2 c 2 ) > 16.7 (20) [4] So, the formula for flexural rigidity D is then reduced to: D = Ef ( btd2 2 ) (21) [4] As a mentioned earlier this is almost the same case as sixsection module and when applying the parallel axis theorem, one would expect the same calculations and results. So, the expectation is that the rigidity at the outer layers contributes with a higher amount of flexural rigidity than the inner layers when considering the entire sandwich structure Deflection of Beams This section deals with beam deflection. Deflection occurs when a specified load is applied to a cross section beam, and the amount of deflection and stress are very important to determine for sandwich structures and beams, for example in case of sandwich, as the core has a relatively low shear modulus, and the beam may deflect a considerable amount due to shear deformations, to neglect the proper consideration of the shear modulus of the core may lead to unconservative prediction of deflections or critical loads. [11] In addition, it is very important to know the limits of deflections for sandwich structure beams to ensure the integrity and stability of a structure or to prevent any attached brittle materials from cracking Therefore, it is essential to determine the modulus and take its effect into account. [19] 35
36 The deflection of beams depends mostly on the modulus of elasticity of the chosen material and must occur within the elastic limit of the material. They are determined using the elastic theory. There is always some additional deflection in the material due to shear, but it is normally so small that it can be neglected. Figure below illustrates the deflection and curvature due to bending. [11] Figure 2.16 Deflection and curvature due to bending [20] There are different types of supports for example supports that resist a force like a pin or a displacement, another supports for instance resist a moment like a fixed end support, resist displacement or a rotation [20]. The following examples illustrate the deflection of a cantilever and a simply supported beam. [21, pp ] Cantilever beam: A cantilever beam is when a beam is attached at only one end and free on the other end as shown in figure below. [21, pp ] Figure 2.17 Cantilever beam [20] The deflection for a cantilever beam at any section in terms of x at free end is given by: And the maximum deflection at the free end is: Y = Fx2 6EI (3L x) (22) 36
37 Y max = FL3 3EI (23) When the load F is concentrated at any point as shown below, then the deflection is: Y = Fx2 (3a x) for 0 < x < a 6EI (24) And the maximum deflection in this case is: Y = Fa2 (3x a) for a < x < L 6EI Y max = Fa2 3EI (3L a) (25) When the load is constant and uniformly distributed (W), then the deflection is: Y = Wx2 24EI (x2 + 6L 2 4Lx) (26) And the maximum deflection in this case is: Y max = WL4 8EI (27) When the load is variable but still uniformly distributed then the deflection is: Y = W 0x 2 120LEI (10L3 10L 2 x + 5Lx 2 x 3 ) (28) Similarly, the maximum deflection in this case is: Y max = W 0L 4 30EI (29) For the couple moment M at the free end of the beam, we have: And maximum is: Y = Mx2 2EI Y max = ML2 2EI (30) (31) 37
38 Where, Y = deflection (mm) x = d = distance (m) F = force (N) L = length (m) I = area moment of inertia (m 4 ) E = bending modulus (material property) (Pa) M = bending moment (Nm) W = distributed load (N/m) Simply supported beam: A simply supported beam has pinned support at one end and a roller support at the other end. In figure 2.17 below represents the pinned end and B the roller end. [21, pp ] Figure 2.18 Simply supported beam [20] The governing equations of this module are very similar to the previous case when it comes to types of loads, location of the loads, etc. A review and brief description of the equations are given and illustrated in figure below. Figure 2.19 Simply supported beam, deflection at center 38
39 Deflection at concentrated load (P = F) at the center is: Y = Fx 12EI [3L2 4 x] for 0 < x < 1 2 (32) [20] And the maximum deflection (δ max = y max ) at the center is: Y max = FL3 48EI (33) [20] Concentrated load F at any point: Y = Fbx 6LEI (L2 x 2 b 2 ) for 0 < x < a (34) Y = Fb 6LEI (L b (x a)3 + (L 2 b 2 )x x 2 ) for a < x < L Maximum deflection at the center: Y max = Fb(L2 b 2 ) 3/2 9 3LEI at x = (L 2 b 2 )/ 3 (35) Y = Fb 48EI (3L2 4b 2 ) at the center if a > b Figure 2.20 Simply supported beam, uniformly distributed load For a uniformly distributed load (ω = W)N/m as shown in figure 2.20 above, then equations are: Y = Wx 24EI (L3 2Lx 2 x 3 ) (36) 39
40 Maximum deflection: Y max = 5WL4 384EI (37) When the load is uniform and variable, then deflection can be expressed as: Y = When the couple moment M is at the right end, then: And the maximum is: Where, Y = deflection (mm) x = d = distance (m) F = force (N) L = length (m) Y max = I = area moment of inertia (m 4 ) E = bending modulus (material property) (Pa) M = bending moment (Nm) b = width (m) W = distributed load (N/m) W 0x 360LEI (7L4 10L 2 x 2 + 3x 4 ) (38) Y = MLx x2 (1 6EI L 2 ) (39) ML2 9 3EI at x = 1/ 3 (40) 40
41 3 METHOD For the practical part and laboratory experiments of this thesis work, the following module, software, and concepts are considered. 1. Composite Compressive Strength Modeler (CCSM) 2. A case of a solid UD lamina 3. Sandwich structure 4. ThreePoint and FourPoint bending 5. Data analysis 3.1 Composite Compressive Strength Modeler (CCSM) According to User s Manual of CCSM modeler, it deals with many different aspects of beams and plates in terms of deflection, flexural rigidity, etc. Some of the main features of this software include classical laminate theory, stressstrain analysis, failure prediction for composite plates, and a very useful userexpandable database to store material and geometrical properties. However, in this thesis work the modeler is used for determining the stiffness and compliance matrices of beams when sufficient information about the beams, lamina, stiffness, etc. are given. [22] In this thesis work when stiffness and compliance matrices are considered using CCSM modeler the flexural rigidity D will be calculated using width (b) and d 11. And in this case, it is: D theory = b d 11 (41) [22] A Solid UD Lamina A lamina is a building block of modern composites laminated structures, a lamina is also known as a ply or a layer and in our case the UD lamina refers to a unidirectional lamina since each lamina may have more than one type of fibers and these fibers may be oriented in different directions, different thickness, fiber orientation angle and matrix material. [22] 41
42 The geometry of a laminate is normally layers that have three planes of material that are symmetric. Therefore, they exhibit orthotropic behavior (having three mutually perpendicular planes of elastic symmetry at each point). When a lamina cut cross these planes of symmetry, they will exhibit the same mechanical properties. Lines which are normal to these planes of material symmetry are called material axes which are designed as 1, 2, and 3 they are also known as principal material directions. Figure 3.1 below illustrate these axes in a UD lamina. [22] Figure 3.1 Principal material axes in a UD lamina [24] When dealing with fibers, matrix and lamina, it should be mentioned that fibers strength and stiffness are significantly larger than that of the matrix, a lamina is stiffest and strongest in longitudinal direction which is the 0degree direction and they are very weak in the 90degree direction because the load must be carried by the much weaker polymeric matrix. A lamina s mechanical properties in any direction lying in the 23 planes are quite similar and therefore, a unidirectional lamina is considered as transversely isotropic. Each layer has approximately the same properties inplane but different properties through the thickness. [23] 3.2 Bending Bend testing also known as flex or flexural testing is commonly performed to measure the flexural strength and modulus of all types of materials and products. The bending of a material or product can be tested using a bending machining tool. [24] 42
43 A universal bending machine consists of a basic machine that can be adjusted and used for a variety of bends. The basic machine consists of a CNCoperated (computer numerically controlled), a work bench and a software for programming and operating. There are three key analysis when performing bend testing which are, the flexural modulus that deals with measuring slope, stressstrain curve, and stiffness of materials, flexural strength which measures the maximum force that a material can resist before it breaks or yields, and yield point of a material, it is a point at which the material can t restore its normal shape after it. [24] ThreePoint & FourPoint Bending Flexural rigidity, modulus of elasticity and other related quantities can be determined when the values of ThreePoint bending are given. The advantage of using threepoint flexural test is the ease of the specimen preparation and testing. Therefore, the threepoint bending will be the module in the practical part of this thesis work. [25] The fourpoint bending flexural test is very similar to the threepoint bending test. The major difference is the addition of a 4 th bearing, which brings a much larger portion of the beam to the maximum stress. This difference needs to be taken into account when studying for example the brittle materials, since it can be used to indicate the flexural strength and crack initiation for instance, in case of asphalt mixtures that are used in road paving, however the fourpoint bending test won t be included in the practical part of this scientific discourse. [26] 43
44 Tables below show some international standard testing methods. Table 2. ASTM standards for threepoint bend. [27] ASTM ASTMC1161 ASTMC1341 ASTMC1684 ASTMC203 ASTMC473 ASTMC598 ASTMC674 ASTMD1184 ASTMD143 ASTMD2344 ASTMD3044 ASTMD349 ASTMD4476 ASTMD7264 ASTMD790 ASTME855 ASTMF1575 ASTMF Standard Test Method Flexural Strength of Advanced Ceramics at Ambient Temperature Flexural Properties of Continuous Fiber Reinforced Advanced Ceramic Composites Flexural Strength of Advanced Ceramics at Ambient TemperatureCylindrical Rod Strength Breaking Load and Flexural Properties of BlockType Thermal Insulation Physical Testing of Gypsum Panel Products Annealing Point and Strain Point of Glass by Beam Bending for Flexural Properties of Ceramic White Ware Materials form Flexural Strength of Adhesive Bonded Laminated Assemblies Small Clear Specimens of Timber for ShortBeam Strength of Polymer Matrix Composite Materials and Their Laminates Shear Modulus of WoodBased Structural Panels Laminated Round Rods Used for Electrical Insulation Flexural Properties of Fiber Reinforced Pultruded Plastic Rods Flexural Properties of Polymer Matrix Composite Materials Flexural Properties of Unreinforced and Reinforced Plastics and Electrical Insulating Materials Bend Testing of Metallic Flat Materials for Spring Applications Involving Static Loading Determining Bending Yield Moment of Nails Components Used in the Surgical Fixation of the Spinal Skeletal System 44
45 Table 3. ASTM standards for fourpoint bend. [27] ASTM ASTMC1161 ASTMC1341 ASTMC1368 ASTMC1576 ASTMC158 ASTMC1674 ASTMC1684 ASTMC393 ASTMC480 ASTMC651 ASTMD6272 ASTMD7249 ASTMD7264 ASTMD790 ASTME855 Standard Test Method Flexural Strength of Advanced Ceramics at Ambient Temperature Flexural Properties of Continuous Fiber Reinforced Advanced Ceramic Composites Determination of Slow Crack Growth Parameters of Advanced Ceramics by Constant StressRate Strength Testing at Ambient Temperature Determination of Slow Crack Growth Parameters of Advanced Ceramics by Constant Stress Flexural Testing (Stress Rupture) at Ambient Temperature Strength of Glass Flexure (Determination of Modulus of Rupture) Flexural Strength of Advanced Ceramics with Engineered Porosity (Honeycomb Cellular Channels) at Ambient Temperatures Flexural Strength of Advanced Ceramics at Ambient TemperatureCylindrical Rod Strength Core Shear Properties of Sandwich Constructions by Beam Flexure Flexure Creep of Sandwich Constructions Flexural Strength of Manufactured Carbon and Graphite Articles Using FourPoint Loading at Room Temperature Flexural Properties of Unreinforced and Reinforced Plastics and Electrical Insulating Materials by FourPoint Facing Properties of Sandwich Constructions by Long Beam Flexure Flexural Properties of Polymer Matrix Composite Materials Flexural Properties of Unreinforced and Reinforced Plastics and Electrical Insulating Materials Bend Testing of Metallic Flat Materials for Spring Applications Involving Static Loading 45
46 4 RESULTS This section deals with the results, graphs, CCSM modeler, experiments, and data analysis in both theoretical and experimental cases as below. 4.1 Bending Test and CCSM Modelling In this section the goal is to make a comparative analysis between theoretical and experimental flexural rigidity D on a solid fiberglass and a sandwich beam with different orientations using the material testing machine under threepoint bending with a uniform constant load and the CCSM modeler for the theoretical part. Figure 4.1 Materials testing machine 46
47 A solid beam of 10 plies and a sandwich beam of 4 plies are used as examples to obtain the theoretical results of stiffness and compliance matrices for zero degree [0º] using the software package CCSM modeler. The CCSM modeler program can be used by entering the obtained geometry of the beam, that is, the required beam dimensions, save ply data in the input and then calculate for elastic properties according to the user s manual. It should be mentioned that for the sake of time saving and ease of use the same lamina properties and thickness can be saved and used for other layers as long as they are of the same material. However, when the lamina is of different material then the reentering data of each lamina along with corresponding properties is required. 1. Theoretical test solid fiberglass (CCSM modeler): The module in this example as mentioned earlier is symmetric and all layers are made of same material (fiberglass). Both theoretical and experimental tests are applied to this module according to the values given in the table below. Table 4. Values for the CCSM Modeler. Property Symbol Unit Width b 25 mm Thickness (unidirection) ta 0.75 mm Longitudinal modulus E GPa Transverse direction E GPA Poisson number Nu 0.3 Shear Modulus G12 2.1GPa Angle 0 47
48 The first step is to enter the above data to the CCSM modeler. Figure 4.2 Solid fiberglass  theoretical The data used in this example are taken from a real lamina tested in the laboratory using a microscope. So, the data are almost exact. After running the software, the following results are obtained, and we are mainly interested in the d11 value that will be used in determining the value of flexural rigidity. Figure 4.3 Solid fiberglass theoretical d 11 48
49 Based on the CCSM modeler the value of d11 and knowing the total thickness of the lamina, that is: b = 25 mm d 11 = So, the theoretical flexural rigidity is: [22] D theory = b(mm) 25 Nmm2 = 1000 = 32 Nmm d 11 (Nm) The flexural rigidity D theory of the 10 layers fiber glass plies is according to the result above is 32 Nmm Experimental test solid fiberglass: This test is performed in the laboratory using material testing machine model M 3503CT available at Arcada laboratory. The same exact solid beam along with the same exact data are used for this experimental test for the sake of comparison between the theoretical and experimental tests and determining the effectiveness and accuracy of CCSM modeler. Figure below shows the linear elasticity and the slope which is of main interest in calculating flexural rigidity Y (Linear) F (N) y = x R² = X Figure 4.4 Solid fiberglass  experimental 49
50 The experimental calculations of flexural rigidity D are as follows: Slope = df dy = k = 48D L 3 (42) [22] Where, L = length between supports k = Slope = N mm Rearranging the equation 50 leads to: D exp = k L3 48 = k (300mm)3 48 D exp = [ N mm ] [mm3 1 ] = Nmm 2 D exp 31 Nmm 2 The relative error is 1 D exp = 1 31 = 1 0,96875, corresponding to 3.1% D theory Theoretical test sandwich beam (number 1): This example is a sandwich beam with four plies and width of 13mm total, with a 1.5mm width for each face and the longitudinal modulus in this example is assumed 15.5 GPa based on the obtained experimental results of this example as shown in figure 4.5 below. 50
51 Figure 4.5 Sandwich beam 1  theoretical After entering the required data and running the simulation, the following results are obtained as shown below. Figure 4.6 Sandwich beam 1 theoretical d 11 In a similar way to the first case, the theoretical flexural rigidity can be calculated as follows: D theory = b(mm) 100 Nmm2 = 1000 = 155 Nmm2 d 11 (Nm)
52 2. Experimental test sandwich beam (number 1): In this laboratory test a sandwich beam made of core cell M80 and the facings made of vinyl ester is used and the other material properties and constants are taken from table 5 page F [N] y = x R² = Figure 4.7 Sandwich beam 1  experimental Applying the flexural rigidity equation again with the obtained slope k, then: D exp = k L3 48 = k (300mm)3 48 D exp = [ N mm ] [mm3 1 ] = Nmm 2 D exp = 153,3 Nmm 2 The relative error is 1 D exp = 1 153,3 = 1 0, , corresponding to 1,1% D theory
53 1. Theoretical test sandwich beam (number 2): The sandwich beam in this test differs from the previous one by angle of orientation, otherwise all the material, data, dimensions are the same. Figure below shows a screenshot of CCSM modeler with entered data. For convenience and suitability, the longitudinal modulus E11 is taken 50 GPa in this test in order to meet the results obtained from the experimental part, since the slope of the linear elasticity gets much smaller in this case due to orientation of the sandwich beam under threepoint bending. Figure 4.8 Sandwich beam 2  theoretical After running CCSM modeler software, then the following results are obtained for compliance matrix d11. Figure 4.9 Sandwich beam 2 theoretical d 11 53
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationSERVICEABILITY OF BEAMS AND ONEWAY SLABS
CHAPTER REINFORCED CONCRETE Reinforced Concrete Design A Fundamental Approach  Fifth Edition Fifth Edition SERVICEABILITY OF BEAMS AND ONEWAY SLABS A. J. Clark School of Engineering Department of Civil
More informationMATERIALS. Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle?
MATERIALS Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: A. Composition
More informationUnit III Theory of columns. Dr.P.Venkateswara Rao, Associate Professor, Dept. of Civil Engg., SVCE, Sriperumbudir
Unit III Theory of columns 1 Unit III Theory of Columns References: Punmia B.C.,"Theory of Structures" (SMTS) Vol II, Laxmi Publishing Pvt Ltd, New Delhi 2004. Rattan.S.S., "Strength of Materials", Tata
More informationCHAPTER 6 BENDING Part 1
Ishik University / Sulaimani Civil Engineering Department Mechanics of Materials CE 211 CHAPTER 6 BENDING Part 11 CHAPTER 6 Bending Outlines of this chapter: 6.1. Chapter Objectives 6.2. Shear and
More informationMECHANICS OF MATERIALS. Prepared by Engr. John Paul Timola
MECHANICS OF MATERIALS Prepared by Engr. John Paul Timola Mechanics of materials branch of mechanics that studies the internal effects of stress and strain in a solid body. stress is associated with the
More informationMaterials: engineering, science, processing and design, 2nd edition Copyright (c)2010 Michael Ashby, Hugh Shercliff, David Cebon.
Modes of Loading (1) tension (a) (2) compression (b) (3) bending (c) (4) torsion (d) and combinations of them (e) Figure 4.2 1 Standard Solution to Elastic Problems Three common modes of loading: (a) tie
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationFlexure: Behavior and Nominal Strength of Beam Sections
4 5000 4000 (increased d ) (increased f (increased A s or f y ) c or b) Flexure: Behavior and Nominal Strength of Beam Sections Moment (kipin.) 3000 2000 1000 0 0 (basic) (A s 0.5A s ) 0.0005 0.001 0.0015
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationBeam Bending Stresses and Shear Stress
Beam Bending Stresses and Shear Stress Notation: A = name or area Aweb = area o the web o a wide lange section b = width o a rectangle = total width o material at a horizontal section c = largest distance
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More information3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture,
3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture, 09.21.07 1. In the beam considered in PS1, steel beams carried the distributed weight of the rooms above. To reduce stress on the beam, it
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationUnit 15 Shearing and Torsion (and Bending) of Shell Beams
Unit 15 Shearing and Torsion (and Bending) of Shell Beams Readings: Rivello Ch. 9, section 8.7 (again), section 7.6 T & G 126, 127 Paul A. Lagace, Ph.D. Professor of Aeronautics & Astronautics and Engineering
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationFIXED BEAMS IN BENDING
FIXED BEAMS IN BENDING INTRODUCTION Fixed or builtin beams are commonly used in building construction because they possess high rigidity in comparison to simply supported beams. When a simply supported
More informationChapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING )
Chapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING ) 5.1 DEFINITION A construction member is subjected to centric (axial) tension or compression if in any cross section the single distinct stress
More informationLecture 1617, Sandwich Panel Notes, 3.054
Sandwich Panels Two stiff strong skins separated by a lightweight core Separation of skins by core increases moment of inertia, with little increase in weight Efficient for resisting bending and buckling
More informationReview of Strain Energy Methods and Introduction to Stiffness Matrix Methods of Structural Analysis
uke University epartment of Civil and Environmental Engineering CEE 42L. Matrix Structural Analysis Henri P. Gavin Fall, 22 Review of Strain Energy Methods and Introduction to Stiffness Matrix Methods
More informationDEFLECTION OF BEAMS WlTH SPECIAL REFERENCE TO SHEAR DEFORMATIONS
DEFLECTION OF BEAMS WlTH SPECIAL REFERENCE TO SHEAR DEFORMATIONS THE INFLUENCE OF THE FORM OF A WOODEN BEAM ON ITS STIFFNESS AND STRENGTHI (REPRINT FROM NATIONAL ADVISORY COMMITTEE FOR AERONAUTICS REPORT
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationNow we are going to use our free body analysis to look at Beam Bending (W3L1) Problems 17, F2002Q1, F2003Q1c
Now we are going to use our free body analysis to look at Beam Bending (WL1) Problems 17, F00Q1, F00Q1c One of the most useful applications of the free body analysis method is to be able to derive equations
More informationTHE BENDING STIFFNESSES OF CORRUGATED BOARD
AMDVol. 145/MDVol. 36, Mechanics of Cellulosic Materials ASME 1992 THE BENDING STIFFNESSES OF CORRUGATED BOARD S. Luo and J. C. Suhling Department of Mechanical Engineering Auburn University Auburn,
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationModule 4 : Deflection of Structures Lecture 4 : Strain Energy Method
Module 4 : Deflection of Structures Lecture 4 : Strain Energy Method Objectives In this course you will learn the following Deflection by strain energy method. Evaluation of strain energy in member under
More informationtwo structural analysis (statics & mechanics) APPLIED ACHITECTURAL STRUCTURES: DR. ANNE NICHOLS SPRING 2017 lecture STRUCTURAL ANALYSIS AND SYSTEMS
APPLIED ACHITECTURAL STRUCTURES: STRUCTURAL ANALYSIS AND SYSTEMS DR. ANNE NICHOLS SPRING 2017 lecture two structural analysis (statics & mechanics) Analysis 1 Structural Requirements strength serviceability
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationStructural Steelwork Eurocodes Development of A Transnational Approach
Structural Steelwork Eurocodes Development of A Transnational Approach Course: Eurocode Module 7 : Worked Examples Lecture 0 : Simple braced frame Contents: 1. Simple Braced Frame 1.1 Characteristic Loads
More informationIntroduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams.
Outline of Continuous Systems. Introduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams. Vibrations of Flexible Strings. Torsional Vibration of Rods. BernoulliEuler Beams.
More informationMechanical Design in Optical Engineering
OPTI Buckling Buckling and Stability: As we learned in the previous lectures, structures may fail in a variety of ways, depending on the materials, load and support conditions. We had two primary concerns:
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationCivil Engineering Design (1) Design of Reinforced Concrete Columns 2006/7
Civil Engineering Design (1) Design of Reinforced Concrete Columns 2006/7 Dr. Colin Caprani, Chartered Engineer 1 Contents 1. Introduction... 3 1.1 Background... 3 1.2 Failure Modes... 5 1.3 Design Aspects...
More informationMoment of Inertia and Centroid
Chapter Moment of nertia and Centroid Page 1. Moment of nertia and Centroid Theory at a Glance (for ES, GATE, PSU).1 Centre of gravity: The centre of gravity of a body defined as the point through which
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationMECHANICAL PROPERTIES OF SOLIDS
Chapter Nine MECHANICAL PROPERTIES OF SOLIDS MCQ I 9.1 Modulus of rigidity of ideal liquids is (a) infinity. (b) zero. (c) unity. (d) some finite small nonzero constant value. 9. The maximum load a wire
More informationTESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
More information4. SHAFTS. A shaft is an element used to transmit power and torque, and it can support
4. SHAFTS A shaft is an element used to transmit power and torque, and it can support reverse bending (fatigue). Most shafts have circular cross sections, either solid or tubular. The difference between
More informationMECH 401 Mechanical Design Applications
MECH 401 Mechanical Design Applications Dr. M. O Malley Master Notes Spring 008 Dr. D. M. McStravick Rice University Updates HW 1 due Thursday (11708) Last time Introduction Units Reliability engineering
More informationEE C245 ME C218 Introduction to MEMS Design
EE C245 ME C218 Introduction to MEMS Design Fall 2007 Prof. Clark T.C. Nguyen Dept. of Electrical Engineering & Computer Sciences University of California at Berkeley Berkeley, CA 94720 Lecture 16: Energy
More informationAn Evaluation and Comparison of Models for Maximum Deflection of Stiffened Plates Using Finite Element Analysis
Marine Technology, Vol. 44, No. 4, October 2007, pp. 212 225 An Evaluation and Comparison of Models for Maximum Deflection of Stiffened Plates Using Finite Element Analysis Lior Banai 1 and Omri Pedatzur
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationMINIMUM WEIGHT STRUCTURAL SANDWICH
U.S. DEPARTMENT OF AGRICULTURE FOREST SERVICE FOREST PRODUCTS LABORATORY MADISON, WIS. In Cooperation with the University of Wisconsin U.S.D.A. FOREST SERVICE RESEARCH NOTE Revised NOVEMBER 1970 MINIMUM
More informationSize Effects In the Crushing of Honeycomb Structures
45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference 1922 April 2004, Palm Springs, California AIAA 20041640 Size Effects In the Crushing of Honeycomb Structures Erik C.
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More information11 Locate the centroid of the plane area shown. 12 Determine the location of centroid of the composite area shown.
Chapter 1 Review of Mechanics of Materials 11 Locate the centroid of the plane area shown 650 mm 1000 mm 650 x 1 Determine the location of centroid of the composite area shown. 00 150 mm radius 00 mm
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationElasticity: Term Paper. Danielle Harper. University of Central Florida
Elasticity: Term Paper Danielle Harper University of Central Florida I. Abstract This research was conducted in order to experimentally test certain components of the theory of elasticity. The theory was
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationDiscontinuous Distributions in Mechanics of Materials
Discontinuous Distributions in Mechanics of Materials J.E. Akin, Rice University 1. Introduction The study of the mechanics of materials continues to change slowly. The student needs to learn about software
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationFinite Element Analysis Prof. Dr. B. N. Rao Department of Civil Engineering Indian Institute of Technology, Madras. Module  01 Lecture  11
Finite Element Analysis Prof. Dr. B. N. Rao Department of Civil Engineering Indian Institute of Technology, Madras Module  01 Lecture  11 Last class, what we did is, we looked at a method called superposition
More informationLECTURE 14 Strength of a Bar in Transverse Bending. 1 Introduction. As we have seen, only normal stresses occur at cross sections of a rod in pure
V. DEMENKO MECHNCS OF MTERLS 015 1 LECTURE 14 Strength of a Bar in Transverse Bending 1 ntroduction s we have seen, onl normal stresses occur at cross sections of a rod in pure bending. The corresponding
More informationPLATE GIRDERS II. Load. Web plate Welds A Longitudinal elevation. Fig. 1 A typical Plate Girder
16 PLATE GIRDERS II 1.0 INTRODUCTION This chapter describes the current practice for the design of plate girders adopting meaningful simplifications of the equations derived in the chapter on Plate Girders
More informationChapter 7: Bending and Shear in Simple Beams
Chapter 7: Bending and Shear in Simple Beams Introduction A beam is a long, slender structural member that resists loads that are generally applied transverse (perpendicular) to its longitudinal axis.
More informationJob No. Sheet No. Rev. CONSULTING Engineering Calculation Sheet. Member Design  Steel Composite Beam XX 22/09/2016
CONSULTING Engineering Calculation Sheet jxxx 1 Member Design  Steel Composite Beam XX Introduction Chd. 1 Grade 50 more common than Grade 43 because composite beam stiffness often 3 to 4 times non composite
More informationSERVICEABILITY LIMIT STATE DESIGN
CHAPTER 11 SERVICEABILITY LIMIT STATE DESIGN Article 49. Cracking Limit State 49.1 General considerations In the case of verifications relating to Cracking Limit State, the effects of actions comprise
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More informationDesign of reinforced concrete sections according to EN and EN
Design of reinforced concrete sections according to EN 199211 and EN 19922 Validation Examples Brno, 21.10.2010 IDEA RS s.r.o. South Moravian Innovation Centre, U Vodarny 2a, 616 00 BRNO tel.: +420511
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationEARTHQUAKE SIMULATION TESTS OF BRIDGE COLUMN MODELS DAMAGED DURING 1995 KOBE EARTHQUAKE
EARTHQUAKE SIMULATION TESTS OF BRIDGE COLUMN MODELS DAMAGED DURING 1995 KOBE EARTHQUAKE J. Sakai 1, S. Unjoh 2 and H. Ukon 3 1 Senior Researcher, Center for Advanced Engineering Structural Assessment and
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 4 Pure Bending
EA 3702 echanics & aterials Science (echanics of aterials) Chapter 4 Pure Bending Pure Bending Ch 2 Aial Loading & Parallel Loading: uniform normal stress and shearing stress distribution Ch 3 Torsion:
More informationDETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1
PERIODICA POLYTECHNICA SER. CIV. ENG. VOL. 46, NO. 1, PP. 125 148 (2002) DETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1 Nándor LIEGNER Department of Highway and Railway Engineering
More informationFLEXURE OF STRUCTURAL SANDWICH CONSTRUCTION
FLEXURE OF STRUCTURAL SANDWICH CONSTRUCTION December 1951 INFORMATION REVIEWED AND REAFFIRMED 1958 LOAN COPY Please return to: Wood Engineering Research Forest Products Laboratory Madison, Wisconsin 53705
More informationPhysical Properties Testing Technical Bulletin
Technical Bulletin MANUFACTURER Raven Lining Systems 13105 E. 61 st Street, Suite A Broken Arrow, OK 74012 (918) 6150020 TENSILE TESTING OF PLASTICS ASTM D638, ISO 527 Tensile tests measure the force
More informationChapter 2: Deflections of Structures
Chapter 2: Deflections of Structures Fig. 4.1. (Fig. 2.1.) ASTU, Dept. of C Eng., Prepared by: Melkamu E. Page 1 (2.1) (4.1) (2.2) Fig.4.2 Fig.2.2 ASTU, Dept. of C Eng., Prepared by: Melkamu E. Page 2
More informationMECHANICS OF SOLIDS Credit Hours: 6
MECHANICS OF SOLIDS Credit Hours: 6 Teaching Scheme Theory Tutorials Practical Total Credit Hours/week 4 0 6 6 Marks 00 0 50 50 6 A. Objective of the Course: Objectives of introducing this subject at second
More informationModule 7 Design of Springs. Version 2 ME, IIT Kharagpur
Module 7 Design of Springs Lesson 1 Introduction to Design of Helical Springs Instructional Objectives: At the end of this lesson, the students should be able to understand: Uses of springs Nomenclature
More informationBridge deck modelling and design process for bridges
EURussia Regulatory Dialogue Construction Sector Subgroup 1 Bridge deck modelling and design process for bridges Application to a composite twingirder bridge according to Eurocode 4 Laurence Davaine
More informationChapter 12 Plate Bending Elements. Chapter 12 Plate Bending Elements
CIVL 7/8117 Chapter 12  Plate Bending Elements 1/34 Chapter 12 Plate Bending Elements Learning Objectives To introduce basic concepts of plate bending. To derive a common plate bending element stiffness
More informationAPPENDIX A Thickness of Base Metal
APPENDIX A Thickness of Base Metal For uncoated steel sheets, the thickness of the base metal is listed in Table A.1. For galvanized steel sheets, the thickness of the base metal can be obtained by subtracting
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationSeismic design of bridges
NATIONAL TECHNICAL UNIVERSITY OF ATHENS LABORATORY FOR EARTHQUAKE ENGINEERING Seismic design of bridges Lecture 3 Ioannis N. Psycharis Capacity design Purpose To design structures of ductile behaviour
More informationBasic and Special Design Concepts of CLT Elements loaded outofplane
1 Basic and Special Design Concepts of CLT Elements loaded outofplane G. Schickhofer *, A. Thiel **, J. Dröscher * * Institute of Timber Engineering and Wood Technology, Graz University of Technology
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationBOOK OF COURSE WORKS ON STRENGTH OF MATERIALS FOR THE 2 ND YEAR STUDENTS OF THE UACEG
BOOK OF COURSE WORKS ON STRENGTH OF MATERIALS FOR THE ND YEAR STUDENTS OF THE UACEG Assoc.Prof. Dr. Svetlana LilkovaMarkova, Chief. Assist. Prof. Dimitar Lolov Sofia, 011 STRENGTH OF MATERIALS GENERAL
More informationJournal of Composite Materials. Behaviour of hollow pultruded GFRP square beams with different shear spantodepth ratios
Behaviour of hollow pultruded GFRP square beams with different shear spantodepth ratios Journal: Manuscript ID: Draft Manuscript Type: Original Manuscript Date Submitted by the Author: n/a Complete List
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationEE C245 ME C218 Introduction to MEMS Design Fall 2010
EE C245 ME C218 Introduction to MEMS Design Fall 2010 Prof. Clark T.C. Nguyen Dept. of Electrical Engineering & Computer Sciences University of California at Berkeley Berkeley, CA 94720 Lecture EE C245:
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationLab Exercise #3: Torsion
Lab Exercise #3: Prelab assignment: Yes No Goals: 1. To evaluate the equations of angular displacement, shear stress, and shear strain for a shaft undergoing torsional stress. Principles: testing of round
More informationInitial Stress Calculations
Initial Stress Calculations The following are the initial hand stress calculations conducted during the early stages of the design process. Therefore, some of the material properties as well as dimensions
More informationDETERMINATION OF EI FOR PULTRUDED GFRP SHEET PILE PANELS. Abstract
DETERMINATION OF EI FOR PULTRUDED GFRP SHEET PILE PANELS Yixin Shao, Cynthia Giroux and Zeid Bdeir McGill University Montreal, Quebec, Canada Abstract The flexural rigidity, EI, plays an especially important
More informationAPPENDIX D SUMMARY OF EXISTING SIMPLIFIED METHODS
APPENDIX D SUMMARY OF EXISTING SIMPLIFIED METHODS D1 An extensive literature search revealed many methods for the calculation of live load distribution factors. This appendix will discuss, in detail,
More informationMECH 344/X Machine Element Design
1 MECH 344/X Machine Element Design Time: M 14:4517:30 Lecture 2 Contents of today's lecture Introduction to Static Stresses Axial, Shear and Torsional Loading Bending in Straight and Curved Beams Transverse
More informationCOURSE STE6289 Modern Materials and Computations (Moderne materialer og beregninger 7.5 stp.)
Narvik University College (Høgskolen i Narvik) EXAMINATION TASK COURSE STE6289 Modern Materials and Computations (Moderne materialer og beregninger 7.5 stp.) CLASS: Master students in Engineering Design
More informationTangential or Shearing
UNITII PROPERTIES OF MATTER INTRODUCTION Elasticity is a branch of Physics which deals with the elastic property of materials. When an external force is applied to a body, there will be some change in
More informationFor more Stuffs Visit Owner: N.Rajeev. R07
Code.No: 43034 R07 SET1 JAWAHARLAL NEHRU TECHNOLOGICAL UNIVERSITY HYDERABAD II.B.TECH  I SEMESTER REGULAR EXAMINATIONS NOVEMBER, 2009 FOUNDATION OF SOLID MECHANICS (AERONAUTICAL ENGINEERING) Time: 3hours
More informationVIBRATION AND ACOUSTIC PERFORMANCE OF INPLANE HONEYCOMB SANDWICH PANELS
Clemson University TigerPrints All Theses Theses 801 VIBRATION AND ACOUSTIC PERFORMANCE OF INPLANE HONEYCOMB SANDWICH PANELS Xiao Gong Clemson University, xiaog@clemson.edu Follow this and additional
More informationEQUILIBRIUM and ELASTICITY
PH 2211D Spring 2013 EQUILIBRIUM and ELASTICITY Lectures 3032 Chapter 12 (Halliday/Resnick/Walker, Fundamentals of Physics 9 th edition) 1 Chapter 12 Equilibrium and Elasticity In this chapter we will
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More information